Supplementary Material Design and Molecular Modeling of AbirateroneFunctionalized Gold Nanoparticles
Elżbieta U. Stolarczyk1,*, Marta Łaszcz1, Andrzej Leś1, 2, Marek Kubiszewski1, Krzysztof Kuziak1, Katarzyna Sidoryk3, Krzysztof Stolarczyk2
Pharmaceutical Research Institute, R&D Analytical Department, 8 Rydygiera Str.,
01-793 Warsaw, Poland 2
University of Warsaw, Faculty of Chemistry, 1 Pasteura Str., 02-093 Warsaw, Poland
Pharmaceutical Research Institute, Chemistry Department, 8 Rydygiera Str.,
01-793 Warsaw, Poland Author to whom correspondence should be addressed: *
Pharmaceutical Research Institute, R&D Analytical Department, 8 Rydygiera Str., 01-793
Warsaw, Poland, tel. +48 22 456 3992 e-mail: [email protected]
Elements of the validation of the UV-Vis method for the determination of AB residual in the supernatant
Abiraterone UV-Vis spectrum in n-BuOH shows λmax at 255 nm. Linearity: The calibration curve was obtained in the concentration range from 4 µg/mL – 50 µg/mL. For each concentration three repetitions were performed for the average result. Three
replicate injections were made for each concentration and the average result was reported. The response of abiraterone was found to be linear in the investigated concentration range and the linear regression equation was y = 0.028x – 0.0069 with the correlation coefficient equal 0.9997 (Table S1, Figure S1). Table S1. Results of the method linearity test. Linearity of the abiraterone determination Mean Solution Concentration, RSD Abs Abs Absorbance SD Abs No. µg/mL % (Abs)
1.108 1.414 1.414 1.414
0.00 Mean SD RSD
0.028 0.028 0.028 0.028 0.001 1.991
Table: Analysis of the linear regression y = 0.0281x – 0.0069 R2 Number of data Standard deviation SDxy Coefficient a (slope):
0.9997 7.00 0.009
a Standard deviation SDa ta=|a|/SDa tcr (a=0.05: f=n-2) Conclusion
0.028 0.0002 135.16 2.57
ta » tcr Coefficient a is significant, the method is sensitive
Coefficient b (y-intercept): b Standard deviation SDb tb=|b|/SDb tcr(a=0.05: f=n-2) Conclusion
-0.007 0.006 1.183 2.57
tb< tcr Coefficient b is not significant, the method has no systematic errors
Coefficient r: r r sq tr=r/√(1-r^2 )×√(n-2) tcr(a=0.05: f=n-2) Conclusion
tr » tcr Coefficient r is significant, the method is linear
0.9999 0.9997 135.16 2.57
Figure S1. Linearity of the abiraterone determination.
Precision: precision was evaluated by measuring the response of six replicate solutions with the analytes at 50 µg/mL (Table S2). Table S2. Results of the precision test for abiraterone. Sample No.
AB Abs 1.409
1 2 3
The limit of detection (LOD): LOD is defined as the lowest concentration of an analyte that an analytical process can reliably differentiate from the back-ground levels. Solutions of different lowering concentrations of AB were analysed. The limit of quantification (LOQ): LOQ is defined as the lowest concentration of the standard that can be measured with an acceptable precision and linearity. Solutions of different lowering concentrations of AB were analysed. The precision of the LOQ level was established by measuring the response of six replicate measurements of the LOQ solution for AB (Table S3) . Detection and quantification limits were found to be 3 µg/mL and 4 µg /mL, respectively. Table S3. Results for the examined LOQ solutions. Sample No.
2. Theoretical studies The selected geometry parameters are collected in Table S4. An interesting feature of the small Aun clusters is their irregular (non-symmetrical) structure, except for Au20 which is close to a tetrahedral structure.
Table S4. Jmol structures of AB acetate and its complexes with Au clusters. AB
AuNPs–(N)AB acetate for Au5
Jmol structures of AB and its complexes with Au clusters AB
AuNPs–(N)AB for Au5
AuNPs–(N)AB for Au13
AuNPs–(OH)AB for Au13
Footnote to Table S4. Distances between neighbouring atoms, in nm, in the Aun clusters predicted with the present theoretical calculations.
Au20 27.3-32.1 Table S5. Intermolecular interaction energies of the Aun–abiraterone conjugates calculated with the use of the counterpoise correction. The A symbol corresponds to Aun, while the B symbol to the abiraterone molecule (neutral/protonated/acetated) or to its reduced models. Conjugate
Reduced models Au13–(N)pyridine
Charged models [Au5–(NH)abiraterone](+)
-1215.868551 -15.92 -66.6
Aun–abiraterone acetate Au5–(N)abiraterone acetate
Au5–(O=C )abiraterone acetate
-1893.322625 -1892.8487451) -1893.306051 -1892.8487451)
1) The sum of electronic and thermal free energy
2) Calculations using smaller Gaussian basis set D95V  3.
3.1. Abiraterone acetate 3.1.1. XRPD studies The diffractogram of the lyophilized mixture is characterised by sharp peaks in the range of 5 – 35 o and broad peaks in the range of 35 – 85 o (Figure S2). Identification of the crystalline phases in the mixture diffractogram proved that the sharp peaks belong to the AB acetate phase and the broad peaks belong to the Au phase (PDF no 04-0784) . The presence of AB acetate in the mixture is confirmed by the comparison of the mixture diffractogram with a simulated diffractogram of AB acetate . Broad Au peaks indicate small sizes of the crystallites. The FWHM value for the Au (111) peak at 38.2 o is 1.4 o. The average size of the Au crystallites estimated from the Scherrer formula for this peak is about 6 nm.
Meas. data:AuNP-50AB acetate lyophilized mi xture
Simulated diffractogram of AB acetate
Figure S2. Identification of the crystalline phases in the lyophilized mixture.
Upper window: a mixture diffractogram, Au peaks are indicated. Below: the simulated diffractogram of AB acetate, an insert: a magnification of low intensity peaks range. 4. NP-based system 4.1.AuNPs-AB acetate 4.1.1. XRPD Figure S3 shows a diffractogram of the AuNPs–AB acetate conjugate. The lack of the AB acetate diffraction peaks suggests its presence in the amorphous content. Broad Au diffraction peaks are best visible. The FWHM value of the Au (111) peak is 0.6 o. An average size of the Au crystallites estimated from the Scherrer formula for this peak is about 14 nm. 1000 Au
2-theta (deg) Figure S3. A diffractogram of the AuNPs–AB acetate conjugate.
4.1.2. Raman Figure S4 shows a comparison of the theoretical Raman spectra of AB acetate as well as the Au5–(N)AB acetate and Au5–(O)AB acetate conjugate in the range from 1800 to 1000 cm-1. This comparison demonstrates that the same band is observed in the three spectra at
about 1740 cm-1, coming from the C=C (B) stretching vibrations. Substantial differences occur in the ranges of 1700 – 1600 cm-1 and in 1100 – 1000 cm-1. In the spectrum of Au5–(O)AB acetate a characteristic band at 1692 cm-1, originating from the C=O stretching vibrations, is observed. In all studied spectra the band at about 1660 cm-1 comes from the collaborative stretching vibrations of mainly C=C (D) bond and the pyridine ring. The band at about 1640 cm-1 comes from the stretching vibrations of the pyridine ring in the AB acetate spectrum, but in the nanoparticle spectra this band comes from the collaborative vibrations of the pyridine ring and the C=C (D) bond. In the range of 1100–1000 cm-1a very intensive band at 1045 cm-1 is observed , in the spectrum of Au5–(N)AB acetate, originating from the pyridine ring vibrations. In the spectra of AB acetate and Au5–(O)AB acetate the band at 1040 cm-1 comes from the AB acetate molecule vibrations. The description of the spectra is summarised in Table S6.
AB acetate Au5-(N)AB acetate Intensity
Raman shift, [cm-1] Figure S4. A comparison of the theoretical Raman spectra of AB acetate and the nanoparticles of Au5– (N)AB acetate and Au5–(O)AB acetate in the range from 1800 to 1000 cm-1.
Table S6. A description of the characteristic bands in the theoretical spectra of AB acetate and the nanoparticles of Au5–(N)AB acetate and Au5–(O)AB acetate. Au5–(N)AB acetate
Raman shifts, (cm-1) 1824 C=O
1742 C=C (B)
1742 C=C (B)
1742 C=C (B)
1665 mainly C=C (D)
1662 mainly C=C (D)
1641 Pyridine ring
1645 mainly pyridine
1666 mainly C=C (D) + pyridine 1642 mainly pyridine
+ C=C (D)
1076 whole AB acetate molecule
+ C=C (D)
1069 steroid moiety
1076 whole AB acetate
without the pyridine ring 1036 whole AB acetate molecule
1038 whole AB acetate molecule
Experimental Raman spectra of AB acetate and the AuNPs–AB acetate conjugate are compared in Figure S5. The experimental spectrum of AB acetate is similar to the calculated one. The experimental spectrum of the AuNPs–AB acetate conjugate is characterised by very broad bands at about 1579, 1446, 1378, 1310, 1264, and 1142 cm-1. One characteristic intense narrow band at 1028 cm-1 is observed. This band is shifted 4 cm-1 into higher wavenumbers in comparison with its counterpart in the experimental AB acetate spectrum which indicates an interaction between the AuNPs and AB acetate. The direction of this shift agrees well with theoretical predictions, but it is difficult to conclude on the manner of the interaction because the experimental spectrum of AuNPs–AB acetate is characterised by very broad bands in the range of 1800–1500 cm-1.
Figure S5. A comparison of the experimental Raman spectra of AB acetate (red spectrum) and AuNPs– AB acetate (blue spectrum).
Figure S6. TGA curves of AB and the nanoparticles.